data_1000066
_cod_database_code               1010298
_structure_refined               no
_mpod_phase_name                 ?
_mpod_phase_generic_name         Nd:SGGM
_chemical_formula_sum            'Nd0.0136 Sr0.92 Gd1.01 Ga2.88 O7'
_mpod_symmetry_point_group_name_h-m '-4 2 m'
_cell_length_a                   7.972
_cell_length_c                   5.251
loop_
_publ_author_name
'Zhang, Y.Y.'
'Zhang, H.J.'
'Yu, H.H.'
'Wang, J.Y.'
'Gao, W.L.'
'Xu, M.'
'Sun, S.Q.'
'Jiang, M.H.'
'Boughton, R.I.'
_publ_section_title
;
 Synthesis, growth, and characterization of Nd-doped SrGdGa3O7 crystal
;
_journal_name_full               'Journal of Applied Physics'
_journal_volume                  108
_journal_issue                   6
_journal_article_reference       063534
_journal_pages_number            10
_journal_year                    2010
_mpod_phase_density              5634
data_1000066a
loop_
_prop_tensorial_index
_prop_thermal_conductivity_kappaij
_prop_thermal_diffusivity_kappadij
_prop_measurement_method
_prop_conditions_temperature
11 . 0.00000067 LPM 303
22 . 0.00000067 LPM 303
33 . 0.00000059 LPM 303
11 1.59 . LPM 303.1
22 1.59 . LPM 303.1
33 ? . LPM 303.1
11 ? . LPM 304
22 ? . LPM 304
33 1.40 . LPM 304
11 ? . LPM 560.2
22 ? . LPM 560.2
33 1.96 . LPM 560.2
11 2.12 . LPM 560.6
22 2.12 . LPM 560.6
33 ? . LPM 560.6
data_1000066b
loop_
_prop_tensorial_index
_prop_thermal_expansion_alphaij
_prop_measurement_method
_prop_conditions_temperature_range_begin
_prop_conditions_temperature_range_end
11 5.32 SCXD 303 773
22 5.32 SCXD 303 773
33 5.65 SCXD 303 773
data_1000066c
loop_
_prop_tensorial_index
_prop_heat_capacity_C
_prop_measurement_method
_prop_conditions_temperature
. 0.419 DSC 303
data_1000066d
loop_
_prop_tensorial_index
_prop_optical_index_extraordinary_ne
_prop_optical_index_ordinary_no
_prop_measurement_method
_prop_conditions_wavelength
. 2.0616061 2.0379258 MDT 0.2537
. 1.9066923 1.9012401 MDT 0.363
. 1.8864119 1.8793089 MDT 0.4047
. 1.8749420 1.8670582 MDT 0.4358
. 1.8629145 1.8543279 MDT 0.480
. 1.8506377 1.8414330 MDT 0.5461
. 1.8451414 1.8357980 MDT 0.5875
. 1.8393703 1.8296930 MDT 0.6438
. 1.8345550 1.8246548 MDT 0.7065
. 1.8272175 1.8170938 MDT 0.8521
. 1.8222021 1.8118757 MDT 1.014
. 1.8139621 1.8033156 MDT 1.530
. 1.8057108 1.7946656 MDT 2.325
